The effect of pressure on the post-synthetic modification of a nanoporous metal-organic framework.
McKellar, Scott C.; Graham, Alexander J.; Allan, David R.; Mohideen, M Infas H; Morris, Russell E.; Moggach, Stephen A.; Nanoscale 6 (2014) 4163–4173; doi:10.1039/c3nr04161a

data_1514155
_publ_section_title
;
 The effect of pressure on the post-synthetic modification of a nanoporous
 metal-organic framework.
;
_journal_issue                   8
_journal_name_full               Nanoscale
_journal_page_first              4163
_journal_page_last               4173
_journal_paper_doi               10.1039/c3nr04161a
_journal_volume                  6
_journal_year                    2014
_chemical_formula_moiety         'C30 H24 Cu3 O21.(CH3)2CHOH'
_chemical_formula_sum            'C33 H32 Cu3 O22'
_chemical_formula_weight         971.23
_space_group_IT_number           164
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     other
_audit_creation_date             12-10-02
_audit_creation_method           CRYSTALS_ver_14.40
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   18.577(2)
_cell_length_b                   18.577(2)
_cell_length_c                   6.8406(9)
_cell_measurement_reflns_used    1156
_cell_measurement_temperature    293
_cell_measurement_theta_max      16
_cell_measurement_theta_min      2
_cell_volume                     2044.4(4)
_computing_cell_refinement       'USER DEFINED CELL REFINEMENT'
_computing_data_collection       'USER DEFINED DATA COLLECTION'
_computing_data_reduction        'USER DEFINED DATA REDUCTION'
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'USER DEFINED STRUCTURE SOLUTION'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.745
_diffrn_measured_fraction_theta_max 0.743
_diffrn_measurement_device       Area
_diffrn_measurement_device_type  'Rigaku Saturn 724+'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.48590
_diffrn_reflns_av_R_equivalents  0.1356
_diffrn_reflns_limit_h_max       0
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            4771
_diffrn_reflns_theta_full        15.436
_diffrn_reflns_theta_max         15.751
_diffrn_reflns_theta_min         0.865
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.534
_exptl_absorpt_correction_T_max  0.85
_exptl_absorpt_correction_T_min  0.72
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Siemens, 1996)'
_exptl_crystal_colour            crystal
_exptl_crystal_density_diffrn    1.578
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             986
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.100
_platon_squeeze_details
;
see above for details
;
_refine_diff_density_max         0.76
_refine_diff_density_min         -0.74
_refine_ls_extinction_method     None
_refine_ls_goodness_of_fit_ref   0.9858
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     94
_refine_ls_number_reflns         822
_refine_ls_number_restraints     116
_refine_ls_R_factor_all          0.1221
_refine_ls_R_factor_gt           0.0678
_refine_ls_shift/su_max          0.0004119
_refine_ls_shift/su_mean         0.0000092
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 Method= Quasi-Unit weights 
 W = 1.0 or 1./2F 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.2159
_refine_ls_wR_factor_gt          0.1562
_refine_ls_wR_factor_ref         0.2159
_reflns_limit_h_max              0
_reflns_limit_h_min              -17
_reflns_limit_k_max              20
_reflns_limit_k_min              0
_reflns_limit_l_max              7
_reflns_limit_l_min              0
_reflns_number_gt                470
_reflns_number_total             830
_reflns_threshold_expression     I>2.0\s(I)
_oxford_diffrn_Wilson_B_factor   0.00
_oxford_diffrn_Wilson_scale      0.00
_oxford_refine_ls_r_factor_ref   0.1221
_oxford_refine_ls_scale          0.2659(10)
_oxford_reflns_number_all        822
_oxford_reflns_threshold_expression_ref I>-10.0\s(I)
_cod_data_source_file            c3nr04161a2.cif
_cod_data_source_block           st1006
_cod_depositor_comments
;
The following automatic conversions were performed:

'_atom_sites_solution_primary' value 'Other' changed to 'other'
according to
/usr/data/users/saulius/crontab/automatic-downloads/current/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_sg_symbol_H-M      'P -3 m 1 '
_cod_database_code               1514155
_iucr_refine_instruction_details_constraints
;
BLOCK SCALE X'S, U'S 
END                                                                             
;
_iucr_refine_instruction_details_restraints
;
DIST   1.252,.01= O(1) TO C(1) 
DIST   1.427,.01= O(1) TO C(7) 
DIST   1.245,.01= O(2) TO C(6) 
DIST   1.254,.01= O(3) TO C(6) 
DIST   1.476,.01= C(1) TO C(2) 
DIST   1.396,.01= C(2) TO C(3) 
DIST   1.396,.01= C(2) TO C(3,5) 
DIST   1.376,.01= C(3) TO C(4) 
DIST   1.391,.01= C(4) TO C(5) 
DIST   1.497,.01= C(4) TO C(6) 
ANGL 125,1= C(7) TO O(1) TO C(1) 
ANGL 125,1= O(1,5) TO C(1) TO O(1) 
ANGL 118,1= C(2) TO C(1) TO O(1) 
ANGL 118,1= C(2) TO C(1) TO O(1,5) 
ANGL 120,1= C(3) TO C(2) TO C(1) 
ANGL 120,1= C(3,5) TO C(2) TO C(1) 
ANGL 120,1= C(3,5) TO C(2) TO C(3) 
ANGL 120,1= C(4) TO C(3) TO C(2) 
ANGL 120,1= C(5) TO C(4) TO C(3) 
ANGL 120,1= C(6) TO C(4) TO C(3) 
ANGL 120,1= C(6) TO C(4) TO C(5) 
ANGL 121,1= C(4,5) TO C(5) TO C(4) 
ANGL 125,1= O(3) TO C(6) TO O(2) 
ANGL 117,1= C(4) TO C(6) TO O(2) 
ANGL 117,1= C(4) TO C(6) TO O(3) 
REM   HREST   START (DO NOT REMOVE THIS LINE) 
REM   HREST   END (DO NOT REMOVE THIS LINE) 
REM   DELU   START (DO NOT REMOVE THIS LINE) 
VIBR .0, 0.00200 = O(1) TO C(1) 
VIBR .0, 0.00200 = O(1) TO C(7) 
VIBR .0, 0.00500 = C(7) TO C(1) 
VIBR .0, 0.00200 = O(2) TO C(6) 
VIBR .0, 0.00200 = O(3) TO C(6) 
VIBR .0, 0.00200 = C(1) TO C(2) 
VIBR .0, 0.00500 = O(1) TO O(1,5) 
VIBR .0, 0.00500 = C(2) TO O(1,5) 
VIBR .0, 0.00500 = C(2) TO O(1) 
VIBR .0, 0.00200 = C(2) TO C(3,5) 
VIBR .0, 0.00200 = C(2) TO C(3) 
VIBR .0, 0.00500 = C(3,5) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(3,5) 
VIBR .0, 0.00200 = C(3) TO C(4) 
VIBR .0, 0.00500 = C(4) TO C(2) 
VIBR .0, 0.00200 = C(4) TO C(5) 
VIBR .0, 0.00200 = C(4) TO C(6) 
VIBR .0, 0.00500 = C(5) TO C(3) 
VIBR .0, 0.00500 = C(6) TO C(3) 
VIBR .0, 0.00500 = C(6) TO C(5) 
VIBR .0, 0.00500 = C(4) TO C(4,5) 
VIBR .0, 0.00500 = O(2) TO C(4) 
VIBR .0, 0.00500 = O(3) TO C(4) 
VIBR .0, 0.00500 = O(3) TO O(2) 
VIBR .0, 0.00200 = C(7) TO C(7,-6,1,0,0,3) 
VIBR .0, 0.00500 = C(7,-6,1,0,0,3) TO O(1) 
REM   DELU   END (DO NOT REMOVE THIS LINE) 
REM   THERMSIM   START (DO NOT REMOVE THIS LINE) 
U(IJ) .0, 0.04000 = O(1) TO C(1) 
U(IJ) .0, 0.04000 = O(1) TO C(7) 
U(IJ) .0, 0.08000 = O(2) TO C(6) 
U(IJ) .0, 0.08000 = O(3) TO C(6) 
U(IJ) .0, 0.04000 = C(1) TO C(2) 
U(IJ) .0, 0.04000 = C(2) TO C(3,5) 
U(IJ) .0, 0.04000 = C(2) TO C(3) 
U(IJ) .0, 0.04000 = C(3) TO C(4) 
U(IJ) .0, 0.04000 = C(4) TO C(5) 
U(IJ) .0, 0.04000 = C(4) TO C(6) 
U(IJ) .0, 0.04000 = C(7) TO C(7,-6,1,0,0,3) 
REM   THERMSIM   END (DO NOT REMOVE THIS LINE) 
END                                                                             
;